dye-sensitized solar cells: fundamentals and current status ... nano review open access...
Post on 17-Oct-2020
Embed Size (px)
NANO REVIEW Open Access
Dye-Sensitized Solar Cells: Fundamentals and Current Status Khushboo Sharma1, Vinay Sharma2 and S. S. Sharma3*
Dye-sensitized solar cells (DSSCs) belong to the group of thin-film solar cells which have been under extensive research for more than two decades due to their low cost, simple preparation methodology, low toxicity and ease of production. Still, there is lot of scope for the replacement of current DSSC materials due to their high cost, less abundance, and long-term stability. The efficiency of existing DSSCs reaches up to 12%, using Ru(II) dyes by optimizing material and structural properties which is still less than the efficiency offered by first- and second- generation solar cells, i.e., other thin-film solar cells and Si-based solar cells which offer ~ 20–30% efficiency. This article provides an in-depth review on DSSC construction, operating principle, key problems (low efficiency, low scalability, and low stability), prospective efficient materials, and finally a brief insight to commercialization.
Keywords: Dye-sensitized solar cells (DSSCs), Photoanode, Counter electrode, Electrolytes, Metal and metal-free organic dyes, Efficiency, Stability
Introduction Dye-sensitized solar cells (DSSCs) have arisen as a tech- nically and economically credible alternative to the p-n junction photovoltaic devices. In the late 1960s, it was discovered that electricity can be generated through illuminated organic dyes in electrochemical cells. At the University of California at Berkeley, chlorophyll was ex- tracted from spinach (photosynthesis). First chlorophyll- sensitized zinc oxide (ZnO) electrode was synthesized in 1972. For the first time, through electron injection of ex- cited dye molecules into a wide band gap of semicon- ductor, photons were converted into electricity . A lot of research has been done on ZnO-single crystals , but the efficiency of these dye-sensitized solar cells was very poor, as the monolayer of dye molecules was able to absorb incident light only up to 1%. Thus, the effi- ciency was improved by optimizing the porosity of the electrode made up of fine oxide powder, so that the ab- sorption of dye over electrode could be enhanced and as a result light harvesting efficiency (LHE) could also be enhanced. As a result, nanoporous titanium dioxide (TiO2) electrodes with a roughness factor of ca.1000
were discovered, and in 1991, DSSCs with 7% efficiency were invented . These cells, also known as Grätzel cells, were originally co-invented in 1988 by Brian O’Regan and Michael Grätzel at UC Berkeley  and were further developed by the aforementioned scien- tists at Ecole Polytechnique Fédèrale de Lausanne (EPFL) till 1991. Brian O’Regan and Michael Grätzel fabricated a device
based on a 10-μm-thick, high surface area and optically transparent film of TiO2 nanoparticles, coated with a monolayer of a charge transfer dye with ideal spectral characteristics to sensitize the film for light harvesting. The device harvested a high proportion of the incident solar energy flux of 46% and showed exceptionally high efficiencies, even more than 80% efficiencies for the con- version of incident photons to electrical current. The overall incident photon to current conversion efficiency (IPCE) yield was 7.1–7.9% in simulated solar light and 12% in diffuse daylight. A large short circuit current density JSC (greater than 12 mAcm
− 2) and exceptional stability (sustaining at least five million turnovers with- out decomposition) and low cost made the practical ap- plication feasible . In 1993, Grätzel et al. reported 9.6% efficiency of cells, and then in 1997, they achieved 10% at the National Renewable Energy Laboratory (NREL). The sensitizers are usually designed to have functional
* Correspondence: email@example.com 3Department of Physics, Govt. Women Engineering College, Ajmer 305002, India Full list of author information is available at the end of the article
© The Author(s). 2018 Open Access This article is distributed under the terms of the Creative Commons Attribution 4.0 International License (http://creativecommons.org/licenses/by/4.0/), which permits unrestricted use, distribution, and reproduction in any medium, provided you give appropriate credit to the original author(s) and the source, provide a link to the Creative Commons license, and indicate if changes were made.
Sharma et al. Nanoscale Research Letters (2018) 13:381 https://doi.org/10.1186/s11671-018-2760-6
http://crossmark.crossref.org/dialog/?doi=10.1186/s11671-018-2760-6&domain=pdf mailto:firstname.lastname@example.org http://creativecommons.org/licenses/by/4.0/
groups such as –COOH, –PO3H2, and –B(OH)2 for stable adsorption onto the semiconductor substrate [4, 5]. Re- cently in 2018, an efficiency of 8.75% was reported for hy- brid dye-titania nanoparticle-based DSSC for superior low temperature by Costa et al. . In a traditional solar cell, Si provides two functions: acts as source of photoelectrons and provides electric field to separate the charges and cre- ate a current. But, in DSSCs, the bulk of semiconductor is only used as a charge transporter and the photoelectrons are provided by photosensitive dyes. The theoretically pre- dicted power conversion efficiency (PCE) of DSSCs was ap- proximately 20% [7, 8]; thus, an extensive research has been made over the years on DSSCs to improve the effi- ciency and to augment its commercialization. However, in the last few decades, a lot of experiments were carried out to improve the performance of DSSCs. For instance, if one goes through the review articles or papers published around 1920 and 1921, a remarkable difference may be observed in the performance as well as fabrication of these cells. Few re- view papers are discussed below with the objective and main results shown in a respective article to get an idea how the performance of these cells has been improved and, thus, how the DSSCs became a hot topic for researchers. Anandan reviewed the improvements and arising chal-
lenges in dye-sensitized solar cells till 2007 . The main components of his review study were light harvesting in- organic dye molecules, p-CuO nanorod counter elec- trodes, and self-organization of electroactive polymers, and he showed how these materials perform in a ration- ally designed solar cell. However, the maximum IPCE of 7% was discussed in the review paper for naphthyridine coordinated Ru complex  which was good till 2007 but is almost half to the efficiencies shown in later work. The main emphasis of the review paper published by
Bose et al.  was the current state and developments in the field of photoelectrode, photosensitizer, and elec- trolyte for DSSCs till 2015. They have included an inter- esting study of comparing the performance of the DSSC module with that of the Si-based module by the graph shown in Fig. 1  and concluded that the performance of the DSSC module is far better than that of the Si module. Also, the highest efficiency discussed in this re- view paper was 11.2% for N719 dye-based DSSC. Shalini et al.  emphasized on sensitizers, including
ruthenium complexes, metal-free organic dyes, quantum- dot sensitizer, perovskite-based sensitizer, mordant dyes, and natural dyes. However, this article provides a great knowledge about the different types of sensitizers, but lacks the information regarding other important compo- nents of the DSSCs. Again, apart from discussing all dif- ferent components of DSSCs, the review article by Jihuai Wu et al.  was concentrated over the counter elec- trode part. They have discussed the study of different types of counter electrodes based on transparency and
flexibility, metals and alloys, carbon materials, conductive polymers, transition metal compounds, and hybrids. A highest efficiency of 14.3% was discussed for the DSSC fabricated with Au/GNP as a counter electrode, Co3+/2+ as a redox couple, and LEG4 +ADEKA-1 as a sensitizer  and was shown in the review article. Similarly, Yeoh et al. and Fan et al. [16, 17] have given a brief review over the photoanode of DSSC. They have classified modification of photoanode into three categories, namely interfacial modi- fication through the introduction of blocking and scatter- ing layer, compositing, doping with non-metallic anions and metallic cations, interfacial engineering, and replacing the conventional mesoporous semiconducting metal oxide films like with 1-D or 2-D nanostructures. Thus, by comparing different review articles published
earlier, it can be easily seen that the present review art- icle “Dye Sensitized solar Cells: Fundamentals and Current Status” gives the in-depth study of different components and their application in DSSCs as well as construction and working of these cells.
Construction and Working of DSSCs The working electrode, sensitizer (dye), redox-mediator (electrolyte), and counter electrode are four key parame- ters for a DSSC. DSSC is an assembly of working elec- trode soaked with a sensitizer or a dye and sealed to the counter electrode soaked with a thin layer of electrolyte with the help of a hot melt tape to prevent the leakage of the electrolyte (as shown in Fig. 2). The components as well as the construction and working of DSSCs are shown below:
Transparent and Conductive Substrate DSSCs are typically constructed with two sheets of con- ductive transparent materials, which help a substrate for the deposition of the semiconductor and catalyst, acting also as current collectors [18, 19] There are two main
Fig. 1 The performance of dye PV modules increases with temperature, contrary to Si-based modules [(Web reference [available online at http://www.sta.com.au/downloads/DSC%20Booklet